NASA Technical Memorandum

83300 NASA-TM-83300 19820016426

THREE-DIMENSIONAL ANALYSIS OF [0/90]5 AND [9010]5 LAMINATES WITH A CENTRAL CIRCULAR HOLE

Ivatury S. RaJu and John H.

Crew5~

Jr.

Apr; 1 1982

liBRARY COpy (no. ?

'71982

LANGLEY RESEARCH CENTER L1Gr~p.RY,

HAMr~rON.

Nl\SI\

National Aeronautics and Space Adrriinistration Langley Research Center Hampton, Virginia 23665

NASA

VIRGINIA

THREE-DIMENSIONAL ANALYSIS OF [0/90]5 AND [90/0]5 LAMINATES WITH A CENTRAL CIRCULAR HOLE Ivatury S. Raju* and John H. Crews, Jr.** NASA Langley Research Center Hampton, Virginia 23665 SUMMARY Stress

dist~ibutions

[90/0]s laminates, using

were calculated near a circular hole in [0/90]s and

a three-dimensional

finite-element analysis.

stress distributions were presented three ways:

These

through the thickness at the

hole boundary, along radial lines at the 0/90 and 90/0 interfaces, and around the hole at these interfaces. The interlaminar normal stress, az ' and the shear stress, aze' distributions had very steep gradients near the hole boundary, suggesting interlaminar stress singularities.

The largest compres-

sive az stress occurred at about 60° from the load axis; the largest aze occurred near 75°. A simple procedure was introduced to calculate interlaminar stresses near the hole boundary.

It used stresses calculated by an exact

two-dimensional analysis of a laminate with a hole as input to a quasi-threedimensional model.

It produced stresses that agreed closely with. those from

the three-dimensional finite-element model. simple procedure may become

~

For laminates ~ith holes, this

viable alternative to three-dimensional firiite-

element analyses.

*Assistant Research Professor, Joint Institute for Advancement of Flight Sciences, George Washington University at NASA Langley Research Center. ** Senior Engineer.

2

INTRODUCTION Composite laminates are being used extensively in aerospace structures. Many such laminates develop high inter1aminar stresses near holes; such stresses can cause delamination.

•

Unfortunately, the stress state near a cir-

cular hole in a laminate is a complex three-dimensional (3-D) problem. only exact solutions to the problems are two-dimensional (2-D) [1]. literature contains little work on 3-D problems.

The

The

Dana and Barker [2J used the

finite-element method to analyze the stresses around circular holes in [0/90]s' [90/0]s' and [±45]s laminates; they used very coarse models, however.

Experi-

ence with a less complex straight-edge problem [3] showed that coarse models may not yield accurate results near the inter1aminar stress singularity that can exist at the hole boundary.

Tang [4J used a boundary-layer theory to

obtain stress distributions around a circular hole in [0/90]s and [±45J s laminates, but he used an extremely large value of 400 for the ratio of hole radius to ply thickness. One purpose of this paper is to present accurate 3-D stresses for a composite laminate with a more representative ratio of hole radius to the ply thickness.

A second purpose is to introduce a method for estimating the major

inter1aminar stresses near a circular-hole.

The present paper does not pre-

sent design information; instead, it addresses the basic understanding of 3-D stresses at a laminate hole. The present study focused on four-ply laminates with [0/90]s and [90/0]s stacking sequences.

A central circular hole of radius equal to 20 times the

ply thickness was considered.

The laminate had a length-to-widthratio of two,

and the width was six times the hole diameter.

A laminate of such dimensions

3

is, effectively, infinitely wide and long relative to the hole diameter.

This

laminate was analyzed by a finite-element method, like that in Ref. 3, with very high mesh refinement near the intersection of the interface between plies and the hole boundary. The stress distributions are presented in three ways:

through the thick-

ness, along radial lines away from the hole, and around the hole.

Because an

interlaminar stress singularity was expected between the 0° and 90° plies at the hole, the computed stresses were given very near but not at the hole boundary.

Furthermore, the stress magnitudes very near this singularity may

depend on finite-element mesh refinement.

As a result, the peak stresses near

the hole were used only for relative comparisons at different locations around the hole and for relative comparisons among the 3-D stress components at specific points. SY~1BOLS

E••

Young's modulus in i-direction, MPa

G••

shear modulus, MPa

h

ply thickness, m

L

half-length of the laminate, m

R

radius of the circular hole, m

r,a

polar coordinates

"

'J

gross-section stress, MPa u,v,w.

displacements in

w

half-width of the laminate, m

x,y,z

Cartesian coordinates, m

\)

..

lJ

Poisson's ratios

X-,

y-, and z-direction, respectively, m

4

{a}

cylindrical stresses or' 0e' 0z' ore' 0ez' 0zr' MPa

{E}

cylindrical strains Er , Ee , EZ'

Ere'

Eez '

Ezr

Subscripts

,.

i ,j

i,j = 1,2,3

1,2,3

longitudinal, transverse, and thickness directions of a ply

ANALYSIS This section describes the problem analyzed and the corresponding finiteelement model. Laminated Composite Plate with a Circular Hole Fig. 1 shows a four-ply laminate with a half-length of 240h, half-width of 120h, and half-thickness of 2h. radius of 20h.

It has a central circular hole with a

The ends of the laminate were subjected to a uniform displace-

ment in the x-direction.

The gross-section stress necessary for this deforma-

tion was Sg' As previously mentioned, two laminates, [0/90J s and [90/0J s ' were ~on sidered in the analyses. Each ply was idealized as a homogeneous, elastic, orthotropic material with the same properties as in Refs. 3, 5, 6, and 7. Ell

= 138 GPa (20 x 106 psi)

E22

= E33 = 14.5

G12

= G23 = G31 = 5.86 GPa (0.85 x 106 psi)

GPa (2.1 x 106 psi)

The subscripts 1,2, and 3 denote the longitudinal, transverse, and thickness directions,. respectively, of an individual ply.

5

The analysis is aimed at obtaining the stress distribution in the idealized laminate due to the above-mentioned loading, Sg'

Because of the com-

plexity in satisfying the equations of equilibrium, compatibility conditions, and boundary conditions of orthotropic elasticity, exact solutions are not Therefore, approximate methods are being used to obtain the stress

available.

distributions in the laminate.

In the present study, a finite-element analy-

sis based on displacement formulation was used. Because of the symmetries in the problem, only one-eighth of the laminate was analyzed, as shown in Fig. 1. scribed as zero on x x

= 240h

~

The displacements

u,

v, and w were pre-

0, Y = 0, and z = 0 planes, respectively.

plane, a constant displacement u

= Uo

was prescribed.

section stress Sg necessary for this deformation was

On the

The gross-

302u o/h, MPa.

To facilititate presentation of results, a cylindrical coordinate system (r,e,z) was also used.

The stresses in the cylindrical system are shown in

Fig. 1. Finite-Element Idealization One-eighth of the laminate (0

$

x

$

240h,

0

Y $ 120h, and 0

$

was modeled by 20-node isoparametric brick elements.

$

z

$

2h)

The plan view of the.

model is shown in Fig. 2(a) and a 20-noded brick element is shown in Fig. 2(b). The model was subdivided into three regions: region, and a 3-D region. 2-D region.

a 2-D region, a transition

The unshaded region in Fig .. 2(a) corresponds to the

The shaded region very near the hole corresponds to the transi-

tion and the 3-D regions. Fig. 3 shows the through-the-thickness modeling typical of the nine radial lines shown in Fig. 2(a).

The 3-D region extended from 2Gh to 2Gh, the

6

transition was in the region 26h to 27h, and the 2-D region was from 27h onward.

In the 3-D region very near the hole (20h

a polar-type arrangement of elements was used. arrangement of elements very near the hole.

~

r

~

2lh and 0

~

z

~

2h),

The polar mesh had a very fine

This arrangement yields a concen-

tration of stress values very near the intersection of the interface and the hole (z

= h,

r

= R),

where a stress singularity is expected.

A very similar

polar mesh was used in Ref. 3 for a quasi-three-dimensional analysis of the . straight-edge problem in a laminate. The 2-D region extends outward from r

= 27h (see Fig. 3). This 2-D

region. was also modeled by 20-node isoparametric brick elements.

In this

region, one element per ply was used through the thickness and the displacements were assumed to be independent of z. in Fig. 3 had identical

u,

For example, nodes

v, and w displacements.

i,

j, andk

Furthermore, the con-

stitutive relations for the elements in the 2-D region were edited to produce plane stress (oz

= 0)

conditions.

Thus, the 20-node isoparametric brick ele-

ments degenerated to 8-node plane stress quadrilateral elements. The transition elements provided compatibility between the 3-D and 2-D regions.

The transition elements were developed like those reported in

Ref. 8. The element sizes used in the present finite-element modeling are an order of magnitude smaller than the fiber diameters used in current graphite/ epoxy laminates.

Even so, the present analysis was not aimed at idealizing

the fibers and matrix separately, but was aimed at analyzing laminates idealized as consisting of homogeneous, orthotropic plies. were also used in Refs. 2 and 4.

Similar assumptions

7

EVALUATION OF THE FINITE-ELEMENT MODEL The finite-element model for a e

= constant

plane is presented in

Fig. 3. The polar arrangement of elements is much like that used in Ref. 3 to analyze a straight-edge problem involving the same material properties and stacking sequences as the present problem.

Refs. 3 and 7 show that such a

polar mesh gives accurate stresses even near a singularity. Therefore, the present through-the-thickness modeling was expected to be accurate near the interlaminar singularity. Tne modeling around the hole was evaluated by comparing 2-D stress distributions with a known exact solution [1].

Because of the polar arrangement

of elements, the inplane modeling at the midplane (z

= 0)

and the top surface

= 2h) was identical and was coarser than the inplane modeling at the interface (z = h) (see Fig. 3). The inplane modeling at the midplane was used in (z

the 2-D finite-element analysis of a [0/90]s (or [90/0]s) laminate with a hole. Fig. 4 shows the hoop stress lines,

(a e/5 9 ) distribution

on the three radial

e = 0°, 45°, and 90°. The distance from the hole is nondimensional-

ized with the ply thickness.

The solid curves represent 2-D (midplane mesh)

results and the dashed curves represent the exact 2-D solution for an infinite laminate [1]. The two solutions agree closely along all three radial lines. The exact hoop stress ae has a maximum at e = 90° and the corresponding stress-concentration factor, KT, for an infinite laminate is 4.87. For the present finite-element model, the finite width and length elevate the K by about 2.4 percent [9]. Therefore, the exact KT for the present T model is about 4.99. The finite-element solution gave a KT of 4.92, which

8

is only 1.4 percent below the exact value.

~herefore,

even the relatively

coarse midplane modeling predicted the stress distributions accurately. The next parameter to be checked was the extent of the , 3-D r~gion. The quasi-3-D analyses in the literature [3, 5, 6, and 7] show that the 3-D stresses die away within a distance of about 4h from a straight free edge. For the present free-hole problem, two different 3-D models were considered. One model had 3-D elements extending to a distance 6h from the hole (from 20h to 26h), as shown previously in Fig. 3. 3-D region, extending to 4h 3~D

The second model had a smaller

(i.e., from 20h to 24h) from the hole.

The

stresses from both models were nearly identical, showing that either model

was adequate.

The model with the larger 3-D region (20h

throughout the remainder of this study.

~

r

~

26h) was used

This model had about 19,000 degrees

of freedom. Because the finite-element idealization shown in Figs. 2 and 3 can account for the through-the-thickness variations, inplane variations, and 3-D effects, the model was considered accurate and was used to study the stress distribution in the [0/90]s and [90/0]s laminates with a central circular hole.

RESULTS AND DISCUSSION As previously mentioned, stresses are presented first as through-thethickness distributions, next as radial distributions at the interface, and then as circumferential distributions at the interface.

Lastly, estimated

interlaminar stresses based on a procedure described in the Appendix are compared with stresses from the 3-D hole model.

The results for the [0/90]s and

[90/0] . s laminates are presented and discussed together.

9

Through-the-Thickness Distributions Hoop Stress s

83300 NASA-TM-83300 19820016426

THREE-DIMENSIONAL ANALYSIS OF [0/90]5 AND [9010]5 LAMINATES WITH A CENTRAL CIRCULAR HOLE

Ivatury S. RaJu and John H.

Crew5~

Jr.

Apr; 1 1982

liBRARY COpy (no. ?

'71982

LANGLEY RESEARCH CENTER L1Gr~p.RY,

HAMr~rON.

Nl\SI\

National Aeronautics and Space Adrriinistration Langley Research Center Hampton, Virginia 23665

NASA

VIRGINIA

THREE-DIMENSIONAL ANALYSIS OF [0/90]5 AND [90/0]5 LAMINATES WITH A CENTRAL CIRCULAR HOLE Ivatury S. Raju* and John H. Crews, Jr.** NASA Langley Research Center Hampton, Virginia 23665 SUMMARY Stress

dist~ibutions

[90/0]s laminates, using

were calculated near a circular hole in [0/90]s and

a three-dimensional

finite-element analysis.

stress distributions were presented three ways:

These

through the thickness at the

hole boundary, along radial lines at the 0/90 and 90/0 interfaces, and around the hole at these interfaces. The interlaminar normal stress, az ' and the shear stress, aze' distributions had very steep gradients near the hole boundary, suggesting interlaminar stress singularities.

The largest compres-

sive az stress occurred at about 60° from the load axis; the largest aze occurred near 75°. A simple procedure was introduced to calculate interlaminar stresses near the hole boundary.

It used stresses calculated by an exact

two-dimensional analysis of a laminate with a hole as input to a quasi-threedimensional model.

It produced stresses that agreed closely with. those from

the three-dimensional finite-element model. simple procedure may become

~

For laminates ~ith holes, this

viable alternative to three-dimensional firiite-

element analyses.

*Assistant Research Professor, Joint Institute for Advancement of Flight Sciences, George Washington University at NASA Langley Research Center. ** Senior Engineer.

2

INTRODUCTION Composite laminates are being used extensively in aerospace structures. Many such laminates develop high inter1aminar stresses near holes; such stresses can cause delamination.

•

Unfortunately, the stress state near a cir-

cular hole in a laminate is a complex three-dimensional (3-D) problem. only exact solutions to the problems are two-dimensional (2-D) [1]. literature contains little work on 3-D problems.

The

The

Dana and Barker [2J used the

finite-element method to analyze the stresses around circular holes in [0/90]s' [90/0]s' and [±45]s laminates; they used very coarse models, however.

Experi-

ence with a less complex straight-edge problem [3] showed that coarse models may not yield accurate results near the inter1aminar stress singularity that can exist at the hole boundary.

Tang [4J used a boundary-layer theory to

obtain stress distributions around a circular hole in [0/90]s and [±45J s laminates, but he used an extremely large value of 400 for the ratio of hole radius to ply thickness. One purpose of this paper is to present accurate 3-D stresses for a composite laminate with a more representative ratio of hole radius to the ply thickness.

A second purpose is to introduce a method for estimating the major

inter1aminar stresses near a circular-hole.

The present paper does not pre-

sent design information; instead, it addresses the basic understanding of 3-D stresses at a laminate hole. The present study focused on four-ply laminates with [0/90]s and [90/0]s stacking sequences.

A central circular hole of radius equal to 20 times the

ply thickness was considered.

The laminate had a length-to-widthratio of two,

and the width was six times the hole diameter.

A laminate of such dimensions

3

is, effectively, infinitely wide and long relative to the hole diameter.

This

laminate was analyzed by a finite-element method, like that in Ref. 3, with very high mesh refinement near the intersection of the interface between plies and the hole boundary. The stress distributions are presented in three ways:

through the thick-

ness, along radial lines away from the hole, and around the hole.

Because an

interlaminar stress singularity was expected between the 0° and 90° plies at the hole, the computed stresses were given very near but not at the hole boundary.

Furthermore, the stress magnitudes very near this singularity may

depend on finite-element mesh refinement.

As a result, the peak stresses near

the hole were used only for relative comparisons at different locations around the hole and for relative comparisons among the 3-D stress components at specific points. SY~1BOLS

E••

Young's modulus in i-direction, MPa

G••

shear modulus, MPa

h

ply thickness, m

L

half-length of the laminate, m

R

radius of the circular hole, m

r,a

polar coordinates

"

'J

gross-section stress, MPa u,v,w.

displacements in

w

half-width of the laminate, m

x,y,z

Cartesian coordinates, m

\)

..

lJ

Poisson's ratios

X-,

y-, and z-direction, respectively, m

4

{a}

cylindrical stresses or' 0e' 0z' ore' 0ez' 0zr' MPa

{E}

cylindrical strains Er , Ee , EZ'

Ere'

Eez '

Ezr

Subscripts

,.

i ,j

i,j = 1,2,3

1,2,3

longitudinal, transverse, and thickness directions of a ply

ANALYSIS This section describes the problem analyzed and the corresponding finiteelement model. Laminated Composite Plate with a Circular Hole Fig. 1 shows a four-ply laminate with a half-length of 240h, half-width of 120h, and half-thickness of 2h. radius of 20h.

It has a central circular hole with a

The ends of the laminate were subjected to a uniform displace-

ment in the x-direction.

The gross-section stress necessary for this deforma-

tion was Sg' As previously mentioned, two laminates, [0/90J s and [90/0J s ' were ~on sidered in the analyses. Each ply was idealized as a homogeneous, elastic, orthotropic material with the same properties as in Refs. 3, 5, 6, and 7. Ell

= 138 GPa (20 x 106 psi)

E22

= E33 = 14.5

G12

= G23 = G31 = 5.86 GPa (0.85 x 106 psi)

GPa (2.1 x 106 psi)

The subscripts 1,2, and 3 denote the longitudinal, transverse, and thickness directions,. respectively, of an individual ply.

5

The analysis is aimed at obtaining the stress distribution in the idealized laminate due to the above-mentioned loading, Sg'

Because of the com-

plexity in satisfying the equations of equilibrium, compatibility conditions, and boundary conditions of orthotropic elasticity, exact solutions are not Therefore, approximate methods are being used to obtain the stress

available.

distributions in the laminate.

In the present study, a finite-element analy-

sis based on displacement formulation was used. Because of the symmetries in the problem, only one-eighth of the laminate was analyzed, as shown in Fig. 1. scribed as zero on x x

= 240h

~

The displacements

u,

v, and w were pre-

0, Y = 0, and z = 0 planes, respectively.

plane, a constant displacement u

= Uo

was prescribed.

section stress Sg necessary for this deformation was

On the

The gross-

302u o/h, MPa.

To facilititate presentation of results, a cylindrical coordinate system (r,e,z) was also used.

The stresses in the cylindrical system are shown in

Fig. 1. Finite-Element Idealization One-eighth of the laminate (0

$

x

$

240h,

0

Y $ 120h, and 0

$

was modeled by 20-node isoparametric brick elements.

$

z

$

2h)

The plan view of the.

model is shown in Fig. 2(a) and a 20-noded brick element is shown in Fig. 2(b). The model was subdivided into three regions: region, and a 3-D region. 2-D region.

a 2-D region, a transition

The unshaded region in Fig .. 2(a) corresponds to the

The shaded region very near the hole corresponds to the transi-

tion and the 3-D regions. Fig. 3 shows the through-the-thickness modeling typical of the nine radial lines shown in Fig. 2(a).

The 3-D region extended from 2Gh to 2Gh, the

6

transition was in the region 26h to 27h, and the 2-D region was from 27h onward.

In the 3-D region very near the hole (20h

a polar-type arrangement of elements was used. arrangement of elements very near the hole.

~

r

~

2lh and 0

~

z

~

2h),

The polar mesh had a very fine

This arrangement yields a concen-

tration of stress values very near the intersection of the interface and the hole (z

= h,

r

= R),

where a stress singularity is expected.

A very similar

polar mesh was used in Ref. 3 for a quasi-three-dimensional analysis of the . straight-edge problem in a laminate. The 2-D region extends outward from r

= 27h (see Fig. 3). This 2-D

region. was also modeled by 20-node isoparametric brick elements.

In this

region, one element per ply was used through the thickness and the displacements were assumed to be independent of z. in Fig. 3 had identical

u,

For example, nodes

v, and w displacements.

i,

j, andk

Furthermore, the con-

stitutive relations for the elements in the 2-D region were edited to produce plane stress (oz

= 0)

conditions.

Thus, the 20-node isoparametric brick ele-

ments degenerated to 8-node plane stress quadrilateral elements. The transition elements provided compatibility between the 3-D and 2-D regions.

The transition elements were developed like those reported in

Ref. 8. The element sizes used in the present finite-element modeling are an order of magnitude smaller than the fiber diameters used in current graphite/ epoxy laminates.

Even so, the present analysis was not aimed at idealizing

the fibers and matrix separately, but was aimed at analyzing laminates idealized as consisting of homogeneous, orthotropic plies. were also used in Refs. 2 and 4.

Similar assumptions

7

EVALUATION OF THE FINITE-ELEMENT MODEL The finite-element model for a e

= constant

plane is presented in

Fig. 3. The polar arrangement of elements is much like that used in Ref. 3 to analyze a straight-edge problem involving the same material properties and stacking sequences as the present problem.

Refs. 3 and 7 show that such a

polar mesh gives accurate stresses even near a singularity. Therefore, the present through-the-thickness modeling was expected to be accurate near the interlaminar singularity. Tne modeling around the hole was evaluated by comparing 2-D stress distributions with a known exact solution [1].

Because of the polar arrangement

of elements, the inplane modeling at the midplane (z

= 0)

and the top surface

= 2h) was identical and was coarser than the inplane modeling at the interface (z = h) (see Fig. 3). The inplane modeling at the midplane was used in (z

the 2-D finite-element analysis of a [0/90]s (or [90/0]s) laminate with a hole. Fig. 4 shows the hoop stress lines,

(a e/5 9 ) distribution

on the three radial

e = 0°, 45°, and 90°. The distance from the hole is nondimensional-

ized with the ply thickness.

The solid curves represent 2-D (midplane mesh)

results and the dashed curves represent the exact 2-D solution for an infinite laminate [1]. The two solutions agree closely along all three radial lines. The exact hoop stress ae has a maximum at e = 90° and the corresponding stress-concentration factor, KT, for an infinite laminate is 4.87. For the present finite-element model, the finite width and length elevate the K by about 2.4 percent [9]. Therefore, the exact KT for the present T model is about 4.99. The finite-element solution gave a KT of 4.92, which

8

is only 1.4 percent below the exact value.

~herefore,

even the relatively

coarse midplane modeling predicted the stress distributions accurately. The next parameter to be checked was the extent of the , 3-D r~gion. The quasi-3-D analyses in the literature [3, 5, 6, and 7] show that the 3-D stresses die away within a distance of about 4h from a straight free edge. For the present free-hole problem, two different 3-D models were considered. One model had 3-D elements extending to a distance 6h from the hole (from 20h to 26h), as shown previously in Fig. 3. 3-D region, extending to 4h 3~D

The second model had a smaller

(i.e., from 20h to 24h) from the hole.

The

stresses from both models were nearly identical, showing that either model

was adequate.

The model with the larger 3-D region (20h

throughout the remainder of this study.

~

r

~

26h) was used

This model had about 19,000 degrees

of freedom. Because the finite-element idealization shown in Figs. 2 and 3 can account for the through-the-thickness variations, inplane variations, and 3-D effects, the model was considered accurate and was used to study the stress distribution in the [0/90]s and [90/0]s laminates with a central circular hole.

RESULTS AND DISCUSSION As previously mentioned, stresses are presented first as through-thethickness distributions, next as radial distributions at the interface, and then as circumferential distributions at the interface.

Lastly, estimated

interlaminar stresses based on a procedure described in the Appendix are compared with stresses from the 3-D hole model.

The results for the [0/90]s and

[90/0] . s laminates are presented and discussed together.

9

Through-the-Thickness Distributions Hoop Stress s